11.the estimation of the oxide ion polarizability using the electronegativity for b0002www.iiste.org call for paper_o3
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.1, 2012 The Estimation of the Oxide Ion polarizability using the Electronegativity for B2O3-Li2O-Mo glass system El Sayed Moustafa* Farid Elkhateb Faculty of science, Azaher University, physics Department, Assuit Branch, Egypt * E-mail of the corresponding auther:email@example.comAbstract Recently Optical electronegativity of many binary oxide glasses has been evaluated on the basis of twodifferent parameters, the linear refractive index and the energy gap, which have demonstrated remarkablecorrelation. In the present study, an improvement method to estimate the oxide ion polarizability through theaverage optical electronegativity for the lithium borate metal (Mo) glass system has been proposed. Theelectronic oxide polarizability of our prepared ternary oxide glasses have been estimated on the basis of theaverage optical electronegativity. In other side the value of the oxide ion polarizability has been determinedusing the equation of Dimitrov based on the measured linear refractive index.The estimated values are in good agreement with the available experimental data. The present research isanother trend of the oxide ion polarizability determination for ternary glasses.Keywords: oxide ion polarizability , optical electronegativity ,ternary glasses.1- Introduction: One of the most important properties of materials , which is closely related to their applicability in the fieldof optics and electronics, is the electronic polarizability. An estimate of the state of polarization of ions isobtained using the so-called polarizability approach based on the Lorentz –Lorenz equation.Recently oxide glasses take a considerable attention in view of their potential for use as laser hosts, in fiberand as nonlinear optical materials (Varshneya, A.K.,1993, P. Chimalawong et al, 2010).The studies onglasses of metal oxides are relatively meager due to difficulties in identifying and preparing such glassesalthough they show interesting electronic and nonlinear optical properties (Vithal. M.et al. 1997). Thepresent work pertains to some new optical parameters in the case of some ternary glass systems.(Dimitrov.v and Sakka 1996) have shown that for simple oxides, the average electronic oxide polarizabilitycalculated on the basis of two different properties linear refractive index and optical band-gap energyshows remarkable correlation. In the present work we examine whether their observations can be extendedto glasses formed from ternary oxides glasses. This is of a particular interest especially when the relevantquantities can be experimentally obtained for glass systems and polarizability values related to glasses areof value for developing glass systems with nonlinear optical properties. To our knowledge an attempt ofthis kind is being reported for the first time. We chose to lithium borate glass system for our study, as thelithium borates glasses are promising materials have many applications in the electronics components. 25
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.1, 20122- Theoretical considerations:It is well known that the relative ability of an atom to draw electrons in a bond toward itself is called theelectronegativity of the atom. Atoms with large electronegativities (such as F and O) attract the electrons in abond better than those that have small electronegativities (such as Na and Mg). The electronegativities of themain group elements are given by (R. Asokamany and R. manjula,1989) introduced the concept of averageelectronegativity and defined an average electronegativity parameter χ1av in the following manner: N ni χ l χ lav = ∑ ( i =1 N1)Where χ1 is the pauling electronegativity of element, ni is the number of atoms of the ith element and N is thenumber of elements present in the compound. In this connection (R.R. Reddy et al. 2001) have derived thefollowing empirical relationship for the average electronic oxide ion polarizability as follows: αo-2 = 4.624 - 0.7569χlav (2)Where χ1av is the average electronegativity of the simple oxide. Reddy et al have calculated αo2- for manyoxides and in general there is agreement with previously obtained data by Dimitrov. But it should bementioned that polarizability of B2 O3 (2.426A3) and SiO2 (2.419A3) calculated by Equation (2) seems to betoo large.(Reddy.R.R et al. 2001) and (Zhao.X.X et al. 2007) have applied the electronegativity approach to the sameglasses already studied by( Dimitrov.V and Komatsu.T,1999) According to Reddy et al, the followingempirical relations between oxide ion polarizability and average electronegativity is as follows: αo-2 = 4.519 - 0.3422χlav (3) Another formula for all binary oxide glass compositions except TeO2 , GeO2 and TiO2 as a second oxidealso was proposed as follows: αo-2 = ( χlav- 1.35)/( χlav- 1.8) (4) Where χ1av is the average electronegativity of binary oxide glass. On the other hand(Zhao.X.X et al. 2007) have introduced the optical electronegativity calculated from the refractive index topredict oxide ion polarizability of binary oxide glasses. 26
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.1, 2012 αo-2 = 3.5 - 0.9χglass (5)It should be noted that the estimated values of by Reddy et al and zhao et al are in good agreement with therefractive index based oxide ion polarizability of the same glasses obtained by ( Dimitrov.V and Komatsu.T2010 ).Assuming that molar refractivity (Rm) and polarizability αm are additive quantities(Dimitrov and Sakka ,1996) obtained the relationship: R p = pRi + qR O 2− [ = 2.52 pαi + qα O2− ] (6)Where Ri, is ionic refraction of cation, RO2- is the refraction of oxide ion, respectively. P and q denote thenumber of cation and oxide ion in the chemical formula APOq,. This relationship leads to the followingequation: v m (n 2 − 1) α 2 − (n) = [( ) 2 − ∑ pα i ]q −1 (7) o 2.52 (n + 2) iWhere Vm is the molar volume of the glass sample.3- Experimental work: The glass samples were prepared using appropriate amounts of grade reagents boron oxide, lithiumoxide and copper oxide, ferrite oxide zinc, Aluminum and Cadmium oxide. the weighted quantities of thestarting materials for glass batch corresponding to the glass composition were mixed homogeneously. Themixture was placed in a ceramic crucible and heated slowly in an electric furnace to 1100oC. Thetemperature was raised gradually depending upon the glass composition. The crucible containing the meltwas constantly agitated to ensure homogeneous mixing. Sufficient time was allowed for the melt to becomevisibly homogeneous and bubble free. The melt was rapidly quenched to room temperature between twostainless-steel plates. There was no noticeable reaction of the melt with crucible walls. The typical weightloss on melting under the experimental conditions can be neglected with respect to the values quoted for thecomponents. The composition of the glass system was prepared in a series of 6 samples as illustrated intable (1).The density of the samples were measured using Archimedes method using toylene as immersion liquidswith accuracy around ±1%. The samples were annealed at a temperature below glass transition temperature and subsequently polishedwith commercial media and water free lubricant. The glass samples were obtained with a uniform thicknessof 4.0- 5.0 mm. The dc electrical conductivity of prepared glasses, the polished glass samples were silverpainted on both sides and kept in a cell for good contacts. The value of applied voltage =3.0 V and the voltagedrop across the sample and across a standard resistor were measured. Space-charge effects were minimizedby using a very low field, which was applied only briefly. The temperature of the glass sample was measuredby a chromel- alumel ( the measurements have been carried out at room temperature ),thermocouple with anaccuracy of ± 1%. 27
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.1, 2012Also an LCR bridge ( Hioki model 3031, Japan ) was used to carry out the dielectric measurements. Thesamples were coated with silver coatings for obtaining good contact. The accuracy in the measurements ofdielectric constant ε- is ~ ± 0.001 .4- Results:The estimated values of the parameters ( ρ , Vm ,χ1av , αo-2(χ1av), αo-2 ( nm ) and nm) are reported as in table(1 ).Where αo-2 (nm) is the calculated value as a function of the measured refractive index using equation (7),nm is the experimental value according to the dielectric constant. The refractive index has been determinedaccording to the electromagnetic relationship (n=ε1/2 ) in the optical range. αo-2(χ1av) is the obtained value ofoxide ion polarizability according to the average glass electronegativity χ1av which estimated by equation ( 1 ). 5 - Discussions: Considering the data in table ( 2 ), the concept of average electronegativity χ1av can be used to determineand predict the electronic polarizability of the oxide ion for some ternary glasses. The new addition in ourwork is the suggestion of an accurate formula for the calculations of the oxide ion polarizability. Equation(5) is more suitable to obtain αo-2 through χglass with minor change in equation (5) for our samples under test.Accordingly equation ( 5 ) can rewritten as the following: αo-2 = 3.5 - 0.7χlav (9)This formula is more convenience for our system under study, so αo-2 can be evaluated by equation (9).The range of the glass formation in B2O3–Li2O -Mo system extends up to 5 mol % of Mo and all the glasssamples prepared are semi-transparent.The dielectric constant ε, of glasses samples depends on electronic, ionic, and dipole orientation contributionto the polarizability. The ionic polarizability arises from the displacement of ions of opposite sign from theirregular lattice sites , resulting from the applied electric field , as well as from the deformation of theelectronic shells, resulting from the relative of the ions. The behavior of ε our system described may beattributed at low frequency to the polarizability arising from the contribution of multi components in theglassy system. As the frequency increases the ionic and orientation sources of polarizability decreases andfinally disappear due to the inertia of the molecules and ions (S. F. Khor et al,2009). The electronicpolarizability αe is the only process which follows the alternative fields at the visible spectrum. The ionicpolarizability αi, contributes to the polarizability at high frequency. The space charge αs and αo contribute tothe polarizability of the suggested glass system at low frequency. Finally using the the refractive index nm.and the molar volume Vm ,the estimated value of oxide ion polarizability αo-2 , has been evaluated accordingequation ( 7 ) with accurate method.Comparing the two values of αo-2 in table ( 2 ), it is obvious that there is a good agreement between them, thismeans that there are some correlation between the oxide ion polarizability and the electronegativity in thecase of ternary glasses as our samples. 28
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.1, 2012 6-Conclusions:-The oxide ion polarizability has been estimated with more accuracy (± 5% ) for the prepared samples ofternary glasses. It was found that there are a good correlation between the average electronegativity andthe oxide ion polarizability as in the binary systems of glasses at this limit of oxide metal (5mol.% ).- This is a new trial to make a correlation between the electronic polarizability of the oxide ion and theelectronegativity for some ternary glasses as our samples.References:Asokamani. R, Manjula . R, 1989, ( Atomic polarizability and electronegativity for someoxide glasses ),Phys. Rev. B.39, 4217-4221.Dimitrov, V. and T. Komatsu, 1999. (Electronic polarizability, optical basicity and non-linear opticalproperties of oxide glasses ). J. Non-Crystal.Solids, 249: 160-179. DOI: 10.1016/S0023093(99)00317-8.Dimitrov.V and Sakka. S,1996, ( Electronic oxide ion polarizability and optical basicity of simple oxides I ),J. Appl. Phys. 79, 1736.Dimitrov, V. and T. Komatsu, 2010,(An interpretation of optical properties of oxides and oxide glasses interms of the electronic polarizability and avsrage single bond strength), J. Chemi. Technol. Metall., 45,3:219. www.uctm.edu/journal/j2010-3/1_Veselin_Dimitrov_219-250.pdf.S. F. Khor , Z. A. Talib , H. A.A. Sidek , W. M. Daud and B. H. Ng , 2009. ( Effects of ZnO on Dielectric Properties and Electrical Conductivity of Ternary Zinc Magnesium Phosphate Glasses). American Journal of Applied Sciences, 6: 1010-1014.DOI: 10.3844/ajassp.2009.1010.1014.P. Chimalawong , J. Kaewkhao and P. Limsuwan , 2010. Optical Investigation and Electronic Polarizability of Nd3+ Doped Soda-Lime-Silicate Glasses. Energy Research Journal, 1: 176-181. DOI: 10.3844/erjsp.2010.176.181.R.R. Reddy, , Y. Nazeer Ahammed, P. Abdul Azeem, K. Rama Gopal, T.V.R. Rao,2001,( Electronicpolarizability and optical basicity properties of oxide glasses through averageelectronegativity),Vol,286,issue 3,169-180.Doi: 10.1016/S0022-3093(01)00481-1.Varshneya, A.K., 1993. Fundementals of InorganicGlasses. 1st Edn., Academic Press, New YorkISBN-10: 0127149708, pp: 570. 29
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.1, 2012Vithal. M., P. Nachimuthu, T. Banu and R. Jagannathan, 1997. (Optical and Electrical properties ofPbO-TiO2, pbO-TeO2 glass system), J. Appl. Phys., 81: 7923.Doi: 10.1063/1.365366Zhao, X., X. Wang, H. Lin and Z. Wang, 2007. (Correlation among electronic polarizability, optical basicityand interaction parameter of Bismus Borate glasses). Phys. B., 390: 293-300. DOI:10.1016/j.physb.2006.08.047.Table (1) : The prepared samples in mole percent. Ratio in mole% 80 15 5 N0 B2O3 Li2O - (20%) No.1 B2O3 Li2O CuO No. 2 B2O3 Li2O Fe2O3 No. 3 B2O3 Li2O Al2O3 No. 4 B2O3 Li2O ZnO No. 5 B2O3 Li2O CdOTable ( 2 ) illustrates the calculated values of the density , the molar volume,the averageelectronegativity, oxide ion polarizability αo-2(χ1av ) and the oxide ion polarizability as a function of therefractive index of the prepared glasses. Type of glass ρ Vm χ1av αo-2(χ1av) nm g/cm 3 3 cm /mol αo-2(n )m B2O3 – Li2O 2.12 29 3.14 1.304 1.53 1.373 B2O3 – Li2O -CuO 2.20 28.5 3 1.451 1.54 1.365 B2O3 – Li2O -Fe2O3 2.10 29 2.90 1.480 1.51 1.350 B2O3 – Li2O-Al2O3 2.15 29.5 2.80 1.535 1.52 1.355 B2O3 – Li2O-ZnO 2.16 30 2.76 1.550 1.50 1.351 B2O3 – Li2O-CdO 2.14 30 2.70 1.600 1.54 1.352 30
International Journals Call for PaperThe IISTE, a U.S. publisher, is currently hosting the academic journals listed below. The peer review process of the following journalsusually takes LESS THAN 14 business days and IISTE usually publishes a qualified article within 30 days. Authors shouldsend their full paper to the following email address. More information can be found in the IISTE website : www.iiste.orgBusiness, Economics, Finance and Management PAPER SUBMISSION EMAILEuropean Journal of Business and Management EJBM@iiste.orgResearch Journal of Finance and Accounting RJFA@iiste.orgJournal of Economics and Sustainable Development JESD@iiste.orgInformation and Knowledge Management IKM@iiste.orgDeveloping Country Studies DCS@iiste.orgIndustrial Engineering Letters IEL@iiste.orgPhysical Sciences, Mathematics and Chemistry PAPER SUBMISSION EMAILJournal of Natural Sciences Research JNSR@iiste.orgChemistry and Materials Research CMR@iiste.orgMathematical Theory and Modeling MTM@iiste.orgAdvances in Physics Theories and Applications APTA@iiste.orgChemical and Process Engineering Research CPER@iiste.orgEngineering, Technology and Systems PAPER SUBMISSION EMAILComputer Engineering and Intelligent Systems CEIS@iiste.orgInnovative Systems Design and Engineering ISDE@iiste.orgJournal of Energy Technologies and Policy JETP@iiste.orgInformation and Knowledge Management IKM@iiste.orgControl Theory and Informatics CTI@iiste.orgJournal of Information Engineering and Applications JIEA@iiste.orgIndustrial Engineering Letters IEL@iiste.orgNetwork and Complex Systems NCS@iiste.orgEnvironment, Civil, Materials Sciences PAPER SUBMISSION EMAILJournal of Environment and Earth Science JEES@iiste.orgCivil and Environmental Research CER@iiste.orgJournal of Natural Sciences Research JNSR@iiste.orgCivil and Environmental Research CER@iiste.orgLife Science, Food and Medical Sciences PAPER SUBMISSION EMAILJournal of Natural Sciences Research JNSR@iiste.orgJournal of Biology, Agriculture and Healthcare JBAH@iiste.orgFood Science and Quality Management FSQM@iiste.orgChemistry and Materials Research CMR@iiste.orgEducation, and other Social Sciences PAPER SUBMISSION EMAILJournal of Education and Practice JEP@iiste.orgJournal of Law, Policy and Globalization JLPG@iiste.org Global knowledge sharing:New Media and Mass Communication NMMC@iiste.org EBSCO, Index Copernicus, UlrichsJournal of Energy Technologies and Policy JETP@iiste.org Periodicals Directory, JournalTOCS, PKPHistorical Research Letter HRL@iiste.org Open Archives Harvester, Bielefeld Academic Search Engine, ElektronischePublic Policy and Administration Research PPAR@iiste.org Zeitschriftenbibliothek EZB, Open J-Gate,International Affairs and Global Strategy IAGS@iiste.org OCLC WorldCat, Universe Digtial Library ,Research on Humanities and Social Sciences RHSS@iiste.org NewJour, Google Scholar.Developing Country Studies DCS@iiste.org IISTE is member of CrossRef. All journalsArts and Design Studies ADS@iiste.org have high IC Impact Factor Values (ICV).